LMucko/crystallography-open-database huggingface dataset:
Quaternaere Caesium - Kupfer(I) - Lanthanoid(III) - Selenide vom Typ Cs Cu3 M2 Se5 (M = Sm, Gd - Lu)
Strobel, S.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 630 (2004) 706–711; doi:

data_1535236
_publ_section_title
;
 Quaternaere Caesium - Kupfer(I) - Lanthanoid(III) - Selenide vom Typ Cs
 Cu3 M2 Se5 (M = Sm, Gd - Lu)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              706
_journal_page_last               711
_journal_volume                  630
_journal_year                    2004
_chemical_formula_sum            'Cs Cu3 Se5 Tb2'
_chemical_name_systematic        'Cs Cu3 Tb2 Se5'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.1372
_cell_length_b                   14.6875
_cell_length_c                   17.413
_cell_volume                     1058.103
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Strobel_ZAACAB_2004_1376.cif
_cod_data_source_block           Cs1Cu3Se5Tb2
_cod_original_formula_sum        'Cs1 Cu3 Se5 Tb2'
_cod_database_code               1535236
Synthesis and Structural and Spectroscopic Properties of Di-mue-sulphido- and mue-Oxo-mue-sulphido-oxomolybdates(V) with Chloro, Oxalato, and Thio-oxalato Ligands
Mennemann, K.; Mattes, R.; Journal of Chemical Research (Synopsis) 1979 (1979) 100–101; doi:

data_1535237
_publ_section_title
;
 Synthesis and Structural and Spectroscopic Properties of Di-mue-sulphido-
 and mue-Oxo-mue-sulphido-oxomolybdates(V) with Chloro, Oxalato, and
 Thio-oxalato Ligands
;
_journal_name_full               'Journal of Chemical Research (Synopsis)'
_journal_page_first              100
_journal_page_last               101
_journal_volume                  1979
_journal_year                    1979
_chemical_formula_sum            'Cl4 Cs2 H4 Mo2 O4 S2'
_chemical_name_systematic        'Cs2 (S2 Mo2 O2 Cl4 (H2 O)2)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.66
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.781
_cell_length_b                   20.073
_cell_length_c                   10.425
_cell_volume                     1336.279
_citation_journal_id_ASTM        JRPSDC
_cod_data_source_file            Mennemann_JRPSDC_1979_200.cif
_cod_data_source_block           H4Cl4Cs2Mo2O4S2
_cod_original_formula_sum        'H4 Cl4 Cs2 Mo2 O4 S2'
_cod_database_code               1535237
Crystal structure of rhodesite, H K1-x Nax+2y Ca2-y (lB,3,2 2)(Si8 O19) *(6-z)H2O, from three localities and its relation to other silicates with dreier double layers
Hesse, K.F.; Merlino, S.; Liebau, F.; Zeitschrift fuer Kristallographie (149,1979-) 199 (1992) 25–48; doi:

data_8103957
_publ_section_title
;
 Crystal structure of rhodesite, H K1-x Nax+2y Ca2-y (lB,3,2 2)(Si8 O19)
 *(6-z)H2O, from three localities and its relation to other silicates with
 dreier double layers
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              25
_journal_page_last               48
_journal_volume                  199
_journal_year                    1992
_chemical_formula_sum            'Ca2 H11 K O24 Si8'
_chemical_name_systematic        'H K Ca2 Si8 O19 (H2 O)5'
_space_group_IT_number           51
_symmetry_space_group_name_Hall  '-P 2 2a'
_symmetry_space_group_name_H-M   'P m a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   23.4439
_cell_length_b                   6.553
_cell_length_c                   7.055
_cell_volume                     1083.845
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Hesse_ZEKRDZ_1992_34.cif
_cod_data_source_block           H11Ca2K1O24Si8
_cod_original_sg_symbol_Hall     '-P 2a 2a (-x,z,y)'
_cod_original_formula_sum        'H11 Ca2 K1 O24 Si8'
_cod_database_code               8103957
Electrochemical synthesis of perovskite type oxobismuthates (III/V) from hydroxide melts
Bezzenberger, R.; Schoellhorn, R.; European Journal of Solid State Inorganic Chemistry 30 (1993) 435–445; doi:

data_4031585
_publ_section_title
;
 Electrochemical synthesis of perovskite type oxobismuthates (III/V) from
 hydroxide melts
;
_journal_name_full
'European Journal of Solid State Inorganic Chemistry'
_journal_page_first              435
_journal_page_last               445
_journal_volume                  30
_journal_year                    1993
_chemical_formula_sum            'Ba0.65 Bi0.75 K0.31 La0.29 O3'
_chemical_name_systematic        '(K0.31 Ba0.65 La0.04) (La0.25 Bi0.75) O3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.308
_cell_length_b                   4.308
_cell_length_c                   4.308
_cell_volume                     79.952
_citation_journal_id_ASTM        EJSCE5
_cod_data_source_file            Bezzenberger_EJSCE5_1993_852.cif
_cod_data_source_block           Ba0.65Bi0.75K0.31La0.29O3
_cod_original_cell_volume        79.95159
_cod_database_code               4031585
Quaternaere Caesium - Kupfer(I) - Lanthanoid(III) - Selenide vom Typ Cs Cu3 M2 Se5 (M = Sm, Gd - Lu)
Strobel, S.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 630 (2004) 706–711; doi:

data_1535238
_publ_section_title
;
 Quaternaere Caesium - Kupfer(I) - Lanthanoid(III) - Selenide vom Typ Cs
 Cu3 M2 Se5 (M = Sm, Gd - Lu)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              706
_journal_page_last               711
_journal_volume                  630
_journal_year                    2004
_chemical_formula_sum            'Cs Cu3 Se5 Tm2'
_chemical_name_systematic        'Cs Cu3 Tm2 Se5'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.094
_cell_length_b                   14.6619
_cell_length_c                   17.1756
_cell_volume                     1030.979
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Strobel_ZAACAB_2004_1377.cif
_cod_data_source_block           Cs1Cu3Se5Tm2
_cod_original_formula_sum        'Cs1 Cu3 Se5 Tm2'
_cod_database_code               1535238
Structure of an Oxonium Antimony(III) Sulphate, (H3 O)2 Sb2 (S O4)4
Mercier, R.; Douglade, J.; Sheldrick, G.M.; Jones, P.G.; Acta Crystallographica C (39,1983-) 39 (1983) 145–148; doi:

data_2020146
_publ_section_title
;
 Structure of an Oxonium Antimony(III) Sulphate, (H3 O)2 Sb2 (S O4)4
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              145
_journal_page_last               148
_journal_volume                  39
_journal_year                    1983
_chemical_formula_sum            'H3 O9 S2 Sb'
_chemical_name_systematic        '(H3 O) Sb (S O4)2'
_space_group_IT_number           29
_symmetry_space_group_name_Hall  'P 2c -2b'
_symmetry_space_group_name_H-M   'P b c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.085
_cell_length_b                   13.76
_cell_length_c                   8.919
_cell_volume                     1360.412
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            Mercier_ACSCEE_1983_174.cif
_cod_data_source_block           H6O18S4Sb2
_cod_depositor_comments
;

2017-08-31
Z value and formula fixed to values more according to usual
chemical conventions.                 miguel
;
_cod_original_formula_sum            'H6 O18 S4 Sb2'
_cod_original_formula_units_Z            4
_cod_original_cell_volume        1360.411
_cod_original_sg_symbol_Hall     'P 2c -2ac (y,-x,z)'
_cod_database_code               2020146
Wickenburgite, a double-layer silicate Pb3 Al[6](Ca[6] Al[4] Si10[4] O27 (H2 O)3) * (H2 O): crystal chemistry and thermal behaviour
Hesse, K.F.; Liebau, F.; Eulert, H.H.; Zeitschrift fuer Kristallographie (149,1979-) 218 (2003) 542–552; doi:

data_8103958
_publ_section_title
;
 Wickenburgite, a double-layer silicate Pb3 Al[6](Ca[6] Al[4] Si10[4] O27
 (H2 O)3) * (H2 O): crystal chemistry and thermal behaviour
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              542
_journal_page_last               552
_journal_volume                  218
_journal_year                    2003
_chemical_formula_sum            'Al2 Ca H8 O31 Pb3 Si10'
_chemical_name_systematic        'Pb3 Al (Ca Al Si10 O27 (H2 O)3) (H2 O)'
_space_group_IT_number           159
_symmetry_space_group_name_Hall  'P 3 -2c'
_symmetry_space_group_name_H-M   'P 3 1 c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   8.555
_cell_length_b                   8.555
_cell_length_c                   20.19
_cell_volume                     1279.696
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Hesse_ZEKRDZ_2003_982.cif
_cod_data_source_block           H8Al2Ca1O31Pb3Si10
_cod_original_cell_volume        1279.697
_cod_original_formula_sum        'H8 Al2 Ca1 O31 Pb3 Si10'
_cod_database_code               8103958
Electrochemical synthesis of perovskite type oxobismuthates (III/V) from hydroxide melts
Bezzenberger, R.; Schoellhorn, R.; European Journal of Solid State Inorganic Chemistry 30 (1993) 435–445; doi:

data_4031586
_publ_section_title
;
 Electrochemical synthesis of perovskite type oxobismuthates (III/V) from
 hydroxide melts
;
_journal_name_full
'European Journal of Solid State Inorganic Chemistry'
_journal_page_first              435
_journal_page_last               445
_journal_volume                  30
_journal_year                    1993
_chemical_formula_sum            'Ba0.64 Bi0.7 K0.32 Nd0.34 O3'
_chemical_name_systematic        '(K0.32 Ba0.64 Nd0.04) (Nd0.3 Bi0.7) O3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.302
_cell_length_b                   4.302
_cell_length_c                   4.302
_cell_volume                     79.618
_citation_journal_id_ASTM        EJSCE5
_cod_data_source_file            Bezzenberger_EJSCE5_1993_855.cif
_cod_data_source_block           Ba0.64Bi0.7K0.32Nd0.34O3
_cod_database_code               4031586
Quaternaere Caesium - Kupfer(I) - Lanthanoid(III) - Selenide vom Typ Cs Cu3 M2 Se5 (M = Sm, Gd - Lu)
Strobel, S.; Schleid, T.; Zeitschrift fuer Anorganische und Allgemeine Chemie 630 (2004) 706–711; doi:

data_1535239
_publ_section_title
;
 Quaternaere Caesium - Kupfer(I) - Lanthanoid(III) - Selenide vom Typ Cs
 Cu3 M2 Se5 (M = Sm, Gd - Lu)
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              706
_journal_page_last               711
_journal_volume                  630
_journal_year                    2004
_chemical_formula_sum            'Cs Cu3 Se5 Yb2'
_chemical_name_systematic        'Cs Cu3 Yb2 Se5'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.0857
_cell_length_b                   14.6552
_cell_length_c                   17.1204
_cell_volume                     1025.114
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Strobel_ZAACAB_2004_1378.cif
_cod_data_source_block           Cs1Cu3Se5Yb2
_cod_original_formula_sum        'Cs1 Cu3 Se5 Yb2'
_cod_database_code               1535239
Atomic structure of superionic phase of (N H4)3 H (Se O4)2 crystals
Merinov, B.V.; Antipin, M.Yu.; Struchkov, Yu.T.; Tregubchenko, A.M.; Baranov, A.I.; Shuvalov, L.A.; Kristallografiya 36 (1991) 872–875; doi:

data_1535240
_publ_section_title
;
 Atomic structure of superionic phase of (N H4)3 H (Se O4)2 crystals
;
_journal_name_full               Kristallografiya
_journal_page_first              872
_journal_page_last               875
_journal_volume                  36
_journal_year                    1991
_chemical_formula_sum            'H13 N3 O8 Se2'
_chemical_name_systematic        '(N H4)3 H (Se O4)2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   6.052
_cell_length_b                   6.052
_cell_length_c                   22.97
_cell_volume                     728.601
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Merinov_KRISAJ_1991_1161.cif
_cod_data_source_block           H13N3O8Se2
_cod_original_cell_volume        728.6005
_cod_database_code               1535240
Synthesis, structure and magnetic properties of the silicides RE Ir Si (RE = Ce, Pr, Er, Tm, Lu) and Sm Ir0.266(8) Si1.734(8)
Heying, B.; Valldor, M.; Poettgen, R.; Rodewald, U.C.; Hoffmann, R.D.; Mishra, R.; Monatshefte fuer Chemie und verwandte Teile anderer Wissenschaften (109,1978-) 135 (2004) 1335–1347; doi:

data_1535241
_publ_section_title
;
 Synthesis, structure and magnetic properties of the silicides RE Ir Si
 (RE = Ce, Pr, Er, Tm, Lu) and Sm Ir0.266(8) Si1.734(8)
;
_journal_name_full
;
Monatshefte fuer Chemie und verwandte Teile anderer Wissenschaften (109,1978-)
;
_journal_page_first              1335
_journal_page_last               1347
_journal_volume                  135
_journal_year                    2004
_chemical_formula_sum            'Ce Ir Si'
_space_group_IT_number           198
_symmetry_space_group_name_Hall  'P 2ac 2ab 3'
_symmetry_space_group_name_H-M   'P 21 3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.2915
_cell_length_b                   6.2915
_cell_length_c                   6.2915
_cell_volume                     249.036
_citation_journal_id_ASTM        MOCMB7
_cod_data_source_file            Heying_MOCMB7_2004_1491.cif
_cod_data_source_block           Ce1Ir1Si1
_cod_original_cell_volume        249.0363
_cod_original_formula_sum        'Ce1 Ir1 Si1'
_cod_database_code               1535241
Electrochemical synthesis of perovskite type oxobismuthates (III/V) from hydroxide melts
Bezzenberger, R.; Schoellhorn, R.; European Journal of Solid State Inorganic Chemistry 30 (1993) 435–445; doi:

data_4031587
_publ_section_title
;
 Electrochemical synthesis of perovskite type oxobismuthates (III/V) from
 hydroxide melts
;
_journal_name_full
'European Journal of Solid State Inorganic Chemistry'
_journal_page_first              435
_journal_page_last               445
_journal_volume                  30
_journal_year                    1993
_chemical_formula_sum            'Ba0.67 Bi0.68 K0.31 O3 Sm0.34'
_chemical_name_systematic        '(K0.31 Ba0.67 Sm0.02) (Sm0.32 Bi0.68) O3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.289
_cell_length_b                   4.289
_cell_length_c                   4.289
_cell_volume                     78.898
_citation_journal_id_ASTM        EJSCE5
_cod_data_source_file            Bezzenberger_EJSCE5_1993_858.cif
_cod_data_source_block           Ba0.67Bi0.68K0.31O3Sm0.34
_cod_original_cell_volume        78.89839
_cod_database_code               4031587
Muenzmetall-Lanthanid-Chalkogenide:I. Kupfer(I)-Lanthanid(III)-Sulfide der Zusammensetzung Cu M S2(M = La - Nd, Sm, Gd, Tb) im monoklinen A-Typ
Strobel, S.; Lauxmann, P.; Schleid, T.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 60 (2005) 917–923; doi:

data_7222561
_publ_section_title
;
 Muenzmetall-Lanthanid-Chalkogenide:I. Kupfer(I)-Lanthanid(III)-Sulfide
 der Zusammensetzung Cu M S2(M = La - Nd, Sm, Gd, Tb) im monoklinen A-Typ
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              917
_journal_page_last               923
_journal_volume                  60
_journal_year                    2005
_chemical_formula_sum            'Cu S2 Tb'
_chemical_name_systematic        'Cu Tb S2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.214
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.3913
_cell_length_b                   7.0002
_cell_length_c                   6.7046
_cell_volume                     296.889
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Strobel_ZNBSEN_2005_1919.cif
_cod_data_source_block           Cu1S2Tb1
_cod_original_cell_volume        296.8891
_cod_original_formula_sum        'Cu1 S2 Tb1'
_cod_database_code               7222561
Crystal structure of ferroelastic phase II of Cs3H(SeO4)2
Merinov, B.V.; Bolotina, N.B.; Baranov, A.I.; Shuvalov, L.A.; Kristallografiya 36 (1991) 1131–1134; doi:

data_1535242
_publ_section_title
;
 Crystal structure of ferroelastic phase II of Cs3H(SeO4)2
;
_journal_name_full               Kristallografiya
_journal_page_first              1131
_journal_page_last               1134
_journal_volume                  36
_journal_year                    1991
_chemical_formula_sum            'Cs3 H O8 Se2'
_chemical_name_systematic        'Cs3 H (Se O4)2'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-A 2ya'
_space_group_name_H-M_alt        'A 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 102.69
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.037
_cell_length_b                   6.415
_cell_length_c                   16.062
_cell_volume                     1109.448
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Merinov_KRISAJ_1991_1189.cif
_cod_data_source_block           H1Cs3O8Se2
_cod_depositor_comments
;
 Updating space group information.

 Antanas Vaitkus,
 2018-07-23
;
_cod_original_formula_sum        'H1 Cs3 O8 Se2'
_cod_database_code               1535242
Synthesis, structure and magnetic properties of the silicides RE Ir Si (RE = Ce, Pr, Er, Tm, Lu) and Sm Ir0.266(8) Si1.734(8)
Heying, B.; Poettgen, R.; Valldor, M.; Hoffmann, R.D.; Rodewald, U.C.; Mishra, R.; Monatshefte fuer Chemie und verwandte Teile anderer Wissenschaften (109,1978-) 135 (2004) 1335–1347; doi:

data_1535243
_publ_section_title
;
 Synthesis, structure and magnetic properties of the silicides RE Ir Si
 (RE = Ce, Pr, Er, Tm, Lu) and Sm Ir0.266(8) Si1.734(8)
;
_journal_name_full
;
Monatshefte fuer Chemie und verwandte Teile anderer Wissenschaften (109,1978-)
;
_journal_page_first              1335
_journal_page_last               1347
_journal_volume                  135
_journal_year                    2004
_chemical_formula_sum            'Ir0.266 Si1.734 Sm'
_chemical_name_systematic        'Sm Ir0.266 Si1.734'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.093
_cell_length_b                   4.093
_cell_length_c                   13.972
_cell_volume                     234.068
_citation_journal_id_ASTM        MOCMB7
_cod_data_source_file            Heying_MOCMB7_2004_1492.cif
_cod_data_source_block           Ir0.266Si1.734Sm1
_cod_original_formula_sum        'Ir0.266 Si1.734 Sm1'
_cod_database_code               1535243
Electrochemical synthesis of perovskite type oxobismuthates (III/V) from hydroxide melts
Bezzenberger, R.; Schoellhorn, R.; European Journal of Solid State Inorganic Chemistry 30 (1993) 435–445; doi:

data_4031588
_publ_section_title
;
 Electrochemical synthesis of perovskite type oxobismuthates (III/V) from
 hydroxide melts
;
_journal_name_full
'European Journal of Solid State Inorganic Chemistry'
_journal_page_first              435
_journal_page_last               445
_journal_volume                  30
_journal_year                    1993
_chemical_formula_sum            'Ba0.69 Bi0.66 Gd0.35 K0.3 O3'
_chemical_name_systematic        '(K0.3 Ba0.69 Gd0.01) (Gd0.34 Bi0.66) O3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.285
_cell_length_b                   4.285
_cell_length_c                   4.285
_cell_volume                     78.678
_citation_journal_id_ASTM        EJSCE5
_cod_data_source_file            Bezzenberger_EJSCE5_1993_865.cif
_cod_data_source_block           Ba0.69Bi0.66Gd0.35K0.3O3
_cod_original_cell_volume        78.67784
_cod_database_code               4031588
Muenzmetall-Lanthanid-Chalkogenide:I. Kupfer(I)-Lanthanid(III)-Sulfide der Zusammensetzung Cu M S2(M = La - Nd, Sm, Gd, Tb) im monoklinen A-Typ
Strobel, S.; Lauxmann, P.; Schleid, T.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 60 (2005) 917–923; doi:

data_7222562
_publ_section_title
;
 Muenzmetall-Lanthanid-Chalkogenide:I. Kupfer(I)-Lanthanid(III)-Sulfide
 der Zusammensetzung Cu M S2(M = La - Nd, Sm, Gd, Tb) im monoklinen A-Typ
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              917
_journal_page_last               923
_journal_volume                  60
_journal_year                    2005
_chemical_formula_sum            'Ce Cu S2'
_chemical_name_systematic        'Cu Ce S2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.702
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.5869
_cell_length_b                   7.2673
_cell_length_c                   6.8964
_cell_volume                     326.323
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Strobel_ZNBSEN_2005_1920.cif
_cod_data_source_block           Ce1Cu1S2
_cod_original_cell_volume        326.3235
_cod_original_formula_sum        'Ce1 Cu1 S2'
_cod_database_code               7222562